RESIDUAL STRESS EFFECTS IN FRACTURE OF COMPOSITES AND ADHESIVES


 Anna Phebe Caldwell
 2 years ago
 Views:
Transcription
1 RESIDUAL STRESS EFFECTS IN FRACTURE OF COMPOSITES AND ADHESIVES JOHN A. NAIRN ABSTRACT Because composites and adhesive joints are made from different phases with different thermal expansion coefficients, they inevitably develop residual thermal stresses. When designing composites or adhesive joints, it is important to account for these residual stresses. It is not the magnitude of the residual stresses that matters, but rather the effect of those stresses on composite failure properties. This effect can be assessed by including residual stresses in fracture mechanics models of failure. This chapter gives general results for energy release rate in the presence of residual stresses. In many important problems, the effect of residual stress can be evaluated without any need for thermoelasticity analysis of the structure. Several examples of including residual stresses in fracture mechanics interpretation of experimental results are discussed. KEYWORDS Keywords: Residual Stresses, Thermal Stresses, Adhesive Joints, Microcracking, Coatings. INTRODUCTION Composites and structures, such as adhesive joints, are comprised of multiple phases having different thermal expansion coefficients. Because manufacturing methods typically include elevated temperature steps, when the final structure is cooled to use temperature, residual stresses occur. Residual stresses are not necessarily a problem; in some situations they can be beneficial. In other situations, however, residual stresses have an adverse effect on failure properties. Residual stresses may cause a composite to fail sooner than expected, to have greater susceptibility to solvents, or to have reduced durability due to accelerated aging or fatigue damage mechanisms. Thus an important question in all design and analysis with composite materials and adhesive joints is how do residual stresses affect failure properties?
2 This chapter considers fracture mechanics analysis of composites and adhesive joints with residual thermal stresses. The methods here are restricted to structures with linear thermoelastic phases subjected to a uniform change in temperature. Application of fracture mechanics requires evaluation of the energy release rate, G, for propagation of cracks in the presence of residual stresses. In many important problems, the effect of residual stresses on G can be evaluated without the need for any thermoelasticity analysis for residual stresses. This general result makes it possible to easily include residual stress effects in models that previously incorrectly ignored them. The general theory for fracture of structures with residual stresses is given in the theory section. The results section gives some examples of residual stress effects on failure in composites and adhesive joints. THEORY OF RESIDUAL STRESS EFFECTS Consider an arbitrary structure subjected to a uniform temperature change of ΔT and to any mixed traction and displacement boundary conditions as illustrated in Fig. 1. This structure may contain cracks within phases or cracks spanning phases. The goal of any fracture mechanics analysis is to derive the energy release rate for crack growth, which can be calculated from global thermoelastic potential energy using G = dπ da = d(w U) da where Π is the thermoelastic potential energy, W is external work, U is thermoelastic internal energy, and A is crack surface area. By partitioning total stresses into mechanical and residual stresses (σ m and σ r ) and making use of virtual work methods and the divergence theorem, G can be expressed in a useful and general form as (see Refs. [1] and [] for details): G = G mech + VΔT d σ m α da + d σ r α da (1) () where V is total volume and G mech is the energy release rate in the absence of residual stresses: G mech = d 1 T 0 u m ds 1 da S T S u T m u 0 ds (3) The angle brackets indicate volumeaveraged quantities; here they are average mechanical or residual stresses weighted by the phasedependent thermal expansion tensor α. T and u in Eq. (3) are surface tractions and displacements; superscript m indicates the mechanical component of the boundary terms. These results assume traction free crack surfaces and prefect interfaces. The extension of traction loaded cracks and imperfect interfaces is given in Ref. []. The first term in Eq. () is G in the absence of residual stresses; thus the other terms are an exact expression of the residual stress effect in composite fracture. An important special case of Eq. () is to consider mode I fracture. During pure mode I crack growth (and similarly during pure mode II or mode III crack growth) the mode I energy release rate must be proportional to mode I stress intensity factor squared, K I. Furthermore, for linearelastic materials in which all lied tractions and displacements are scaled by a factor P and the temperature difference ΔT
3 Fig. 1: An arbitrary multiphase composite subjected to tractions T 0 on surface S T and displacement boundary conditions u 0 on surface S u and containing crack surfaces (S c ). Fig. : A DCB specimen used to measure mode I toughness of adhesive joints. P is the lied load and a is crack length. is scaled by a factor T *, K I must scale by a linear combination of P and T *. In other words, the mode I energy release rate must have the form G I K I = ( c1 P + c T * ) (4) where c 1 and c are constants that depend on the specific problem. Comparing Eq. (4) to Eq. () and realizing that σ m is proportional to P while σ r is proportional to T *, it is possible to eliminate one term and simplify G I to [1,] G I = G mech 1+ VΔT d σ m α G mech da (5) Notice that G I depends only on mechanical stresses. Thus once the mode I fracture problem is solved ignoring residual stresses, the energy release rate in the presence of residual stresses can be determined exactly without any need for thermoelasticity analysis of the structure. The general result in Eq. (5) has many lications for including residual stress effects in the analysis of fracture of composites and structures. It is analogous to the wellknown Levin [3] analysis that derived a method to exactly calculate effective thermal expansion coefficient of a composite from knowledge of mechanical stresses alone. The Levin analysis used virtual work methods and did not need any thermoelasticity results. Similarly, Eq. (5) was derived with virtual work methods an only needs a mechanical stress analysis. Both analyses are limited to linearelastic materials; Eq. (5) is further limited to pure mode fracture (pure mode I, II, or III), but many important failure problems are pure mode fracture problems. RESIDUAL STRESS EFFECT RESULTS Figure shows a double cantilever beam specimen (DCB) used to measure the fracture toughness of adhesive joints [4]. Assuming the crack runs down the middle of the adhesive as pure mode I fracture, the energy release rate in the presence of residual stresses can be evaluated using Eq. (5) and corrected beam theory to be [5]
4 G I = (C m (a Δ W )P + C r ΔT) (6) where the mechanical and residual constants are given by C m = C κ * B and C r = α * κ C * κ B (7) * Here C κ and * ακ are the simple beam theory compliance and thermal curvature coefficient of one arm of specimen [5], and B is width of the arms. The mechanical term includes an effective crack length (a Δ W ) as discussed elsewhere for corrected beam theory of DCB specimens [5,6]; the coefficient 1.15 on the correction term Δ W [6] was determined numerically by finite element analysis of numerous DCB specimens [5]. The thermal term does not require correction because it is accurate with simple beam theory alone [5]. Comparison to finite element analysis shows that Eq. (6) is accurate within 1% for all adhesive DCB geometries [5]. It is thus easy to correct adhesive tests for residual stress effects. Notice that the residual * stress effect in G I is proportional to α κ, which means the residual stress effect is caused by a tendency of the arms of the specimen to curve due to residual stresses. Many fracture studies on adhesives have ignored residual stresses [4]. Equation (6) can be used to calculate the errors of such an roach [5]. Assume that some particular adhesive has a true fracture toughness of G Ic. If an adhesive DCB specimen with this adhesive is tested, it will fail when G I = G Ic, which, by Eq. (6), hens when the load reaches P = C m G Ic C r ΔT ( ) a +1.15Δ W (8) If this observed failure load is then used in an analysis that ignores residual stresses (i.e., Eq. (6) with ΔΤ=0), the calculated or arent toughness is G Ic = ( GIc C r ΔT ) (9) The difference between G Ic and G Ic is the error caused by ignoring residual stresses. In typical polymer adhesives between metal adherends, C r ΔT is negative which causes G Ic to be higher that the actual toughness. In other words, the presence of residual stresses causes the adhesive to ear tougher than it does without residual stresses. Some sample calculations of errors due to ignoring residual stresses are plotted in Fig. 3 as the percentage error in G Ic as a function of modulus ratio between adherend and adhesive, R, for various adherend to adhesive thickness ratios, λ [5]. The errors are large for low R and λ and decrease as either R or λ increases. The dashed vertical line shows a typical R value for aluminumepoxy specimens. The aluminumepoxy errors exceed 1% even with a very thin adhesive (λ=64) and exceed 40% for a thick adhesive (λ=). A similar analysis [5] can be done for laminate double cantilever beam specimens used to measure delamination toughness. The residual stress effect in DCB specimens can be eliminated by constructing doublysymmetric double cantilever beam specimens in which each arm of the specimen is a symmetric laminate and thus has α * κ = 0. If the arms are not symmetric laminates, however, the residual stress effect can be very large. For example, the errors in G Ic
5 Fig. 3: The percentage error in the arent toughness G Ic in adhesive DCB specimens as a function of adherend to adhesive modulus ratio, R, for various values of adherend to adhesive thickness, λ. The calculations assumed G Ic =00 J/m, Δα =40 X106 K 1, and ΔT = 100 C. The vertical dashed line corresponds to R=8, which is a typical value for aluminumepoxy specimens. for a variety of laminates were calculated to range from 55% to +76% [5]. In other words, the errors caused by ignoring residual stresses can be large and can cause the G Ic result to be either significantly too high or significantly too low. Additional examples of residual stress effects in fracture of composite or structures include matrix microcracking in laminates [7,8], cracking of paints or coatings [9], and interfacial crack growth such as in the microbond or pullout specimens [101]. In matrix microcracking of crossply laminates, the residual stress effect induces tensile stresses in the 90 plies that promote microcracking. The general methods above can include residual stresses in the energy release rate for microcracking; proper analysis of microcracking experiments requires inclusion of the residual stress term. A master plot method is available which make it possible to determine both toughness and residual stress effects from experimental cracking experiments [7,8]. In other words, the value of ΔT in the analysis does not have to be measured or be assumed to be due to linear thermoelastic phases; it can be determined from fracture experiments as an effective ΔT for residual stresses. Cracking of coatings is analogous to microcracking of laminates [9]. An additional source of residual stresses in coatings might arise from chemical shrinkage as the coating cures or dries. Such residual stresses can be included in a thermal stress analysis by replacing thermal strain terms like ΔαΔT by an effective residual strain term due to both chemical and thermal residual stresses [9]. In the microbond specimen [13], a droplet of matrix is deposited on a fiber and an interfacial crack is induced by pulling the fiber while restraining the matrix. In this specimen, all loading is on the top of the droplet while the bottom of the droplet is stress free. A global energy analysis shows that the bulk of the energy released due to crack growth is due to the release of
6 residual stress energy as the droplet and matrix become debonded [10]. Although many interpretations of microbond results have ignored residual stresses, such models have serious errors. By including residual stresses and interfacial friction effects, the microbond specimen can become a fracture mechanics test for determining interfacial mode II fracture toughness [10,14]. For example, it can be used to assess the role of physical aging and residual stress relaxation on interfacial properties [11]. Similar fracture mechanics methods can be used to include residual stress effects in the analysis of singlefiber, pullout experiments [10.1]. RECOMMENDATIONS Residual stresses are always present in composites and structures such as adhesive joints. Proper analysis of fracture experiments with such materials must therefore always include residual stress effects. In some geometries, such as tapered DCB specimens with very large R and λ, residual stresses can be demonstrated to be small and can be ignored [15]. In many important specimens, however, residual stresses are nonnegligible and can even be the dominant effect causing fracture. The methods above give general tools for including residual stresses. These tools assume linear thermoelastic phases with temperatureindependent properties. The general equations can be extended to more general phases and to other sources of residual stresses by replacing ΔT by an effective value that gives the actual level of residual stresses. The use of an effective ΔT usually means the fracture experiments must be coupled with additional experiments that measure the level of residual stresses in the specimen. REFERENCES 1. J. A. Nairn (1997) J. Appl. Mech. 64, J. A. Nairn (000) Int. J. Fract. 105, V. M. Levin (1967) Mechanics of Solids,, S. Mostovoy and E. J. Ripling (1966) J. Appl. Polym. Sci. 10, J. A. Nairn (1999) Int. J. Adhesion & Adhesives 0, J. G. Williams (1995) Proc. Int'l Mechanical Engineering Congress, San Francisco, USA, November J. A. Nairn and S. Hu (1994) in Damage Mechanics of Composite Materials, eds., Ramesh Talreja, J. A. Nairn (000) in Polymer Matrix Composites, eds., R. Talreja and J.Å. E. Manson, S. R. Kim and J. A. Nairn (000) Engr. Fract. Mech. 65, J. A. Nairn (000) Adv. Comp. Letts. 9, S. Zhandarov, E. Pisanova, E. Mader, and J. A. Nairn (000) J. Adhesion Sci. & Tech. 15, D.A. Mendels, Y. Leterrier, J.A. E. Månson, and J. A. Nairn (00) J. Comp. Mat. in press. 13. B. Miller, P. Muri, and L. Rebenfeld (1987) Comp. Sci. & Tech. 8, C. H. Liu and J. A. Nairn (1999) Int. J. Adhesion & Adhesive. 19, B R. K. Blackmand, H. Hadavinia, A. J. Kinloch, M. Paraschi, and J. G. Williams (00) Eng. Fract. Mech. 70,
THE DETERMINATION OF DELAMINATION STRAIN ENERGY RELEASE RATE OF COMPOSITE BIMATERIAL INTERFACE
THE DETERMINATION OF DELAMINATION STRAIN ENERGY RELEASE RATE OF COMPOSITE BIMATERIAL INTERFACE Jaroslav Juracka, Vladimir Matejak Brno University of Technology, Institute of Aerospace Engineering juracka@fme.vutbr.cz;
More informationDistinguishing strength from toughness. Understanding fracture toughness.
Lecture notes version 20 Oct 2010 Chapter 8 Fracture and fracture toughness A fractured Liberty Ship 8.1 Introduction and synopsis Distinguishing strength from toughness. Understanding fracture toughness.
More informationFailure, Analysis and Design. 2003, P. Joyce
Failure, nalysis and esign 23, P. Joyce Special Cases of Laminates The symmetry or antisymmetry of a laminate, based on angle, material, and thickness of plies, may zero out some elements of the three
More informationYield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials. τ xy 2σ y. σ x 3. τ yz 2σ z 3. ) 2 + ( σ 3. σ 3
Yield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials Brittle materials are materials that display Hookean behavior (linear relationship between stress and strain) and which
More informationStructural Integrity Analysis
Structural Integrity Analysis 1. STRESS CONCENTRATION Igor Kokcharov 1.1 STRESSES AND CONCENTRATORS 1.1.1 Stress An applied external force F causes inner forces in the carrying structure. Inner forces
More informationTensile fracture analysis of blunt notched PMMA specimens by means of the Strain Energy Density
Engineering Solid Mechanics 3 (2015) 3542 Contents lists available at GrowingScience Engineering Solid Mechanics homepage: www.growingscience.com/esm Tensile fracture analysis of blunt notched PMMA specimens
More informationMECHANICAL PROPERTIES OF CROSSLAMINATED TIMBER AC COUNTING FOR NONBONDED EDGES AND ADDITIONAL CRACKS
WCTE 6 World Conference on Timber Engineering August 5, 6 Vienna, Austria MECHANICAL PROPERTIES OF CROSSLAMINATED TIMBER AC COUNTING FOR NONBONDED EDGES AND ADDITIONAL CRACKS John A. Nairn ABSTRACT:
More informationThe mode I interlaminar fracture toughness of carbon fiber/epoxy resin composite with freezing after water absorption
High Performance and Optimum Design of Structures and Materials 327 The mode I interlaminar fracture toughness of carbon fiber/epoxy resin composite with freezing after water absorption H. Katogi & K.
More informationMCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions
MCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions The Quiz questions based upon HW9 will open on Thursday, Apr. 11 and close on Wednesday, Apr 17 at 1:30 PM. References to A&J: Chapters 13,
More informationBoundary Conditions in Fluid Mechanics
Boundary Conditions in Fluid Mechanics R. Shankar Subramanian Department of Chemical and Biomolecular Engineering Clarkson University The governing equations for the velocity and pressure fields are partial
More informationInvestigation Of Heat Treating Of Railroad Wheels And Its Effect On Braking Using Finite Element Analysis
Investigation Of Heat Treating Of Railroad Wheels And Its Effect On Braking Using Finite Element Analysis Kexiu Wang Richard Pilon Griffin Wheel Company Abstract This paper studies the heat treatment process
More informationAnalysis of Composite Materials with Abaqus
Analysis of Composite Materials with Abaqus 2016 About this Course Course objectives Upon completion of this course you will be able to: Define anisotropic elasticity for combining the fibermatrix response
More informationFatigue. Figure 41 Typical Comparison of Metal and Composite Fatigue Damage [Salkind, Fatigue of Composites]
Chapter Four PERFORMANCE Fatigue A fundamental problem concerning the engineering uses of fiber reinforced plastics (FRP) is the determination of their resistance to combined states of cyclic stress. [41]
More informationStructural Displacements. Structural Displacements. Beam Displacement. Truss Displacements 2
Structural Displacements Structural Displacements P Beam Displacement 1 Truss Displacements The deflections of civil engineering structures under the action of usual design loads are known to be small
More informationGriffith theory of brittle fracture:
Griffith theory of brittle fracture: Observed fracture strength is always lower than theoretical cohesive strength. Griffith explained that the discrepancy is due to the inherent defects in brittle materials
More informationSimple design method
method Aim of the design method 2 3 Content of presentation in a fire situation method of reinforced concrete slabs at 20 C Floor slab model Failure modes method of at Extension to fire behaviour Membrane
More information8.2 Elastic Strain Energy
Section 8. 8. Elastic Strain Energy The strain energy stored in an elastic material upon deformation is calculated below for a number of different geometries and loading conditions. These expressions for
More informationFatigue :Failure under fluctuating / cyclic stress
Fatigue :Failure under fluctuating / cyclic stress Under fluctuating / cyclic stresses, failure can occur at loads considerably lower than tensile or yield strengths of material under a static load: Fatigue
More informationAdhesion and Viscoelasticity Properties of PVB in Laminated Safety Glass
Adhesion and Viscoelasticity Properties of PVB in Laminated Safety Glass Maurizio FROLI Professor Department of Civil Engineering, Structural Division University of Pisa, Pisa, Italy Maurizio Froli, born
More informationNumerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope
Numerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope Rakesh Sidharthan 1 Gnanavel B K 2 Assistant professor Mechanical, Department Professor, Mechanical Department, Gojan engineering college,
More informationStrength of Concrete
Strength of Concrete In concrete design and quality control, strength is the property generally specified. This is because, compared to most other properties, testing strength is relatively easy. Furthermore,
More informationThermal Diffusivity, Specific Heat, and Thermal Conductivity of Aluminum Oxide and Pyroceram 9606
Report on the Thermal Diffusivity, Specific Heat, and Thermal Conductivity of Aluminum Oxide and Pyroceram 9606 This report presents the results of phenol diffusivity, specific heat and calculated thermal
More informationSECTION 3 Progressive Ply Failure and Delamination Modeling
SECTION 3 Progressive Ply Failure and Delamination Modeling Composites Technology Day, January February 2012 S31 Composites Failure Modeling Look at types of problems you can solve today with MSC s composite
More informationThe Influence of Magnetic Forces on the Stability Behavior of Large Electrical Machines
The Influence of Magnetic Forces on the Stability Behavior of Large Electrical Machines Dr. H. Sprysl, Dr. H. Vögele, ABB Kraftwerke AG, CH5242 Birr Dr. G. Ebi, SENSOPLAN GmbH, D79801 Hohentengen a.h.
More informationComposites: Part A 37 (2006) Short communication
Composites: Part A 37 (2006) 1490 1494 Short communication Discussion on paper The electrical resistance response of continuous carbon fibre composite laminates to mechanical strain by N. Angelidis, C.Y.
More informationDETERMINATION OF TIMETEMPERATURE SHIFT FACTOR FOR LONGTERM LIFE PREDICTION OF POLYMER COMPOSITES
DETERMINATION OF TIMETEMPERATURE SHIFT FACTOR FOR LONGTERM LIFE PREDICTION OF POLYMER COMPOSITES K. Fukushima*, H. Cai**, M. Nakada*** and Y. Miyano*** * Graduate School, Kanazawa Institute of Technology
More informationStress Evolution During and After Deposition of Polycrystalline Thin Films
Stress Evolution During and After Deposition of Polycrystalline Thin Films Carl V. Thompson, Jeff S. Leib, and Hang Yu Dept. of Materials Science and Engineering Massachusetts Institute of Technology Cambridge,
More informationLAP SHEAR STRENGTH OF ADHESIVELY BONDED COMPOSITES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS 1 Introduction LAP SHEAR STRENGTH OF ADHESIVELY BONDED COMPOSITES C. Syn 1, *, S. Gil 1, J. Yoon 1, M. Kim 2 1 Korea Aerospace Industries, 2 The 7
More informationTHERMAL CRACKING RESPONE OF REINFORCED CONCRETE BEAM TO GRADIENT TEMPERATURE
THERMAL CRACKING RESPONE OF REINFORCED CONCRETE BEAM TO GRADIENT TEMPERATURE L. DAHMANI, M.KOUANE Abstract In this paper are illustrated the principal aspects connected with the numerical evaluation of
More informationMechanics of MaterialsSteel
Mechanics of MaterialsSteel Structural Steel Structural steel considered one of the predominant materials for construction of buildings, bridges, towers and other structures. The preferable physical properties
More informationEffect of Heat Treatment Process on the Fatigue Behavior of AISI 1060 Steel
International International Journal of ISSI, Journal Vol. of 12 ISSI, (2015), Vol.10 No.1, (2013), pp. 2832 No.1 Effect of Heat Treatment Process on the Fatigue Behavior of AISI 1060 Steel M. Mehdinia
More informationslip lines which are close to, but not coincident with, the slip lines formed in
FATIGUE CRACK NUCLEATION IN AIETALS* BY T. II. LIN ANI) Y. A11. ITO UNIVERSITY OF CALIFORNIA (LOS ANGELES) Communicated by T'. Y. Thomas, December 18, 1968 Abstract. One of the unanswered questions in
More information(Seattle is home of Boeing Jets)
Dr. Faeq M. Shaikh Seattle, Washington, USA (Seattle is home of Boeing Jets) 1 Pre Requisites for Today s Seminar Basic understanding of Finite Element Analysis Working Knowledge of Laminate Plate Theory
More informationMeasurement of Residual Stress in Plastics
Measurement of Residual Stress in Plastics An evaluation has been made of the effectiveness of the chemical probe and hole drilling techniques to measure the residual stresses present in thermoplastic
More informationCH 6: Fatigue Failure Resulting from Variable Loading
CH 6: Fatigue Failure Resulting from Variable Loading Some machine elements are subjected to static loads and for such elements static failure theories are used to predict failure (yielding or fracture).
More informationINJECTION MOLDING COOLING TIME REDUCTION AND THERMAL STRESS ANALYSIS
INJECTION MOLDING COOLING TIME REDUCTION AND THERMAL STRESS ANALYSIS Tom Kimerling University of Massachusetts, Amherst MIE 605 Finite Element Analysis Spring 2002 ABSTRACT A FEA transient thermal structural
More informationPunching shear behavior of steelconcrete composite decks with different shear connectors
Punching shear behavior of steelconcrete composite decks with different shear connectors *XiaoQing Xu 1) and YuQing Liu 2) 1), 2) Department of Bridge Engineering, Tongji University, Shanghai 200092,
More informationThree dimensional thermoset composite curing simulations involving heat conduction, cure kinetics, and viscoelastic stress strain response
Three dimensional thermoset composite curing simulations involving heat conduction, cure kinetics, and viscoelastic stress strain response Harrison Poon, Seid Koric, M. Fouad Ahmad National Center for
More informationExperimental Study on ZPin Bridging Law by Pullout Test
Experimental Study on ZPin Bridging Law by Pullout Test ShaoCong Dai a, Wenyi Yan, HongYuan Liu a* and YiuWing Mai a a Centre for Advanced Materials Technology (CAMT), School of Aerospace, Mechanical
More informationPlate waves in phononic crystals slabs
Acoustics 8 Paris Plate waves in phononic crystals slabs J.J. Chen and B. Bonello CNRS and Paris VI University, INSP  14 rue de Lourmel, 7515 Paris, France chen99nju@gmail.com 41 Acoustics 8 Paris We
More informationUSE OF CFRP LAMINATES FOR STRENGTHENING OF REINFORCED CONCRETE CORBELS
International Journal of Civil Engineering and Technology (IJCIET) Volume 6, Issue 11, Nov 2015, pp. 1120, Article ID: IJCIET_06_11_002 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=6&itype=11
More informationFatigue crack propagation
1 (20) Repetition Ð Crack initiation and growth Small cracks Shear driven Interact with microstructure Mostly analyzed by continuum mechanics approaches Large cracks Tension driven Fairly insensitive to
More informationTHE IMPACT OF YIELD STRENGTH OF THE INTERCONNECTOR ON THE INTERNAL STRESS OF THE SOLAR CELL WITHIN A MODULE
5th World Conference on Photovoltaic Energy Conversion, 61 September 21, Valencia, Spain THE IMPACT OF YIELD STRENGTH OF THE INTERCONNECTOR ON THE INTERNAL STRESS OF THE SOLAR CELL WITHIN A MODULE Y.
More informationSTRUCTURAL BEHAVIOR OF JOINTS
CHAPTER 5 STRUCTURAL BEHAVIOR OF JOINTS 5.1 INTRODUCTION... 2 5.2 ADHESIVE JOINTS... 3 5.2.1 Introduction... 3 5.2.2 Joint design considerations... 4 5.2.2.1 Effects of adherend thickness: adherend failures
More informationA Study of Durability Analysis Methodology for Engine Valve Considering Head Thermal Deformation and Dynamic Behavior
A Study of Durability Analysis Methodology for Engine Valve Considering Head Thermal Deformation and Dynamic Behavior KumChul, Oh 1, SangWoo Cha 1 and JiHo Kim 1 1 R&D Center, Hyundai Motor Company
More informationValidation of Simulation Results Through Use of DIC Techniques
Validation of Simulation Results Through Use of DIC Techniques Brian Croop and Daniel Roy, DatapointLabs + technical center for materials a DatapointLabs affiliate Materials Testing Data Infrastructure
More informationSTRESSINTENSITY FACTORS BY BOUNDARY COLLOCATION FOR SINGLEEDGENOTCH SPECIMENS SUBJECT TO SPLITTING FORCES. by Bernard Gross and John E.
NASA TECHNICAL NOTE TN D3295.. STRESSINTENSITY FACTORS BY BOUNDARY COLLOCATION FOR SINGLEEDGENOTCH SPECIMENS SUBJECT TO SPLITTING FORCES by Bernard Gross and John E. SrawZey Lewis Research Center
More informationNumerical modelling of shear connection between concrete slab and sheeting deck
7th fib International PhD Symposium in Civil Engineering 2008 September 1013, Universität Stuttgart, Germany Numerical modelling of shear connection between concrete slab and sheeting deck Noémi Seres
More informationObjectives. Experimentally determine the yield strength, tensile strength, and modules of elasticity and ductility of given materials.
Lab 3 Tension Test Objectives Concepts Background Experimental Procedure Report Requirements Discussion Objectives Experimentally determine the yield strength, tensile strength, and modules of elasticity
More informationNew approaches in Eurocode 3 efficient global structural design
New approaches in Eurocode 3 efficient global structural design Part 1: 3D model based analysis using general beamcolumn FEM Ferenc Papp* and József Szalai ** * Associate Professor, Department of Structural
More informationSTRESS AND DEFORMATION ANALYSIS OF LINEAR ELASTIC BARS IN TENSION
Chapter 11 STRESS AND DEFORMATION ANALYSIS OF LINEAR ELASTIC BARS IN TENSION Figure 11.1: In Chapter10, the equilibrium, kinematic and constitutive equations for a general threedimensional solid deformable
More informationInfrared Study of Heat Dissipation under Fatigue Crack Propagation
Infrared Study of Heat Dissipation under Fatigue Crack Propagation O. Plekhov, M. Bannikov, A. erekhina, A. Fedorova Physical foundation of strength Institute of continuous media mechanics RAS str. Ak.
More informationMATHEMATICAL MODEL FOR VIBRATIONS OF NONUNIFORM FLEXURAL BEAMS
Engineering MECHANICS, Vol. 15, 2008, No. 1, p. 3 11 3 MATHEMATICAL MODEL FOR VIBRATIONS OF NONUNIFORM FLEXURAL BEAMS Mohamed Hussien Taha, Samir Abohadima* A simplified mathematical model for free vibrations
More information4 Thermomechanical Analysis (TMA)
172 4 Thermomechanical Analysis 4 Thermomechanical Analysis (TMA) 4.1 Principles of TMA 4.1.1 Introduction A dilatometer is used to determine the linear thermal expansion of a solid as a function of temperature.
More informationEDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME 2 ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS
ENGINEERING COMPONENTS EDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS Structural members: struts and ties; direct stress and strain,
More informationINVESTIGATION INTO FATIGUE BEHAVIOUR OF METALCOMPOSITE GLUE CONNECTION
Fatigue of Aircraft Structures Vol. 1 (2011) 86102 10.2478/v1016401000426 INVESTIGATION INTO FATIGUE BEHAVIOUR OF METALCOMPOSITE GLUE CONNECTION Mirosław Rodzewicz Warsaw University of Technology,
More informationMECHANICS OF SOLIDS  BEAMS TUTORIAL 1 STRESSES IN BEAMS DUE TO BENDING. On completion of this tutorial you should be able to do the following.
MECHANICS OF SOLIDS  BEAMS TUTOIAL 1 STESSES IN BEAMS DUE TO BENDING This is the first tutorial on bending of beams designed for anyone wishing to study it at a fairly advanced level. You should judge
More informationENGI 8673 Subsea Pipeline Engineering Faculty of Engineering and Applied Science
GUIDANCE NOTE LECTURE 12 THERMAL EXPANSION ANALYSIS OVERVIEW The calculation procedure for determining the longitudinal pipeline response can be formulated on the basis of strain. The longitudinal strain
More informationLOADING RATE DEPENDENCY OF COMPLETE STRESSSTRAIN CURVE OF VARIOUS ROCK TYPES
October 1217, 28, Beijing, China ABSTRACT: LOADING RATE DEPENDENCY OF COMPLETE STRESSSTRAIN CURVE OF VARIOUS ROCK TYPES M. Lei 1, K. Hashiba 2, S. Okubo 3 and K. Fukui 4 1 Doctoral student, Dept. of
More informationDifferential Relations for Fluid Flow. Acceleration field of a fluid. The differential equation of mass conservation
Differential Relations for Fluid Flow In this approach, we apply our four basic conservation laws to an infinitesimally small control volume. The differential approach provides point by point details of
More informationFeature Commercial codes Inhouse codes
A simple finite element solver for thermomechanical problems Keywords: Scilab, Open source software, thermoelasticity Introduction In this paper we would like to show how it is possible to develop a
More informationMechanical Properties  Stresses & Strains
Mechanical Properties  Stresses & Strains Types of Deformation : Elasic Plastic Anelastic Elastic deformation is defined as instantaneous recoverable deformation Hooke's law : For tensile loading, σ =
More informationChapter 5 Bridge Deck Slabs. Bridge Engineering 1
Chapter 5 Bridge Deck Slabs Bridge Engineering 1 Basic types of bridge decks Insitu reinforced concrete deck (most common type) Precast concrete deck (minimize the use of local labor) Open steel grid
More informationShort and Large Crack, MixedMode FatigueCrack Growth Thresholds in Ti6Al4V 1
Short and Large Crack, MixedMode FatigueCrack Growth Thresholds in Ti6Al4V 1 Mr. R. K. Nalla, Dr. J. P. Campbell and Professor R. O. Ritchie 2 Department of Materials Science and Engineering University
More informationADHESIVE BONDING PERFORMANCE OF GA COATED 590 MPa TENSILE STRENGTH STEELS
ADHESIVE BONDING PERFORMANCE OF GA COATED 590 MPa TENSILE STRENGTH STEELS Susan Wolf ArcelorMittal Global R&D East Chicago Acknowledgements Chann Cheng, Benda Yan, Jayanth Chintamani, ArcelorMittal Global
More informationMetal films on polymer substrates stretched beyond 50%
Metal films on polymer substrates stretched beyond 50% Nanshu Lu, Xi Wang, Zhigang Suo, Joost Vlassak a School of Engineering and Applied Sciences, Harvard University, Cambridge, MA 02138 Abstract When
More informationDuctile fracture toughness determination,
Xiang (Frank) Chen Randy K. Nanstad, FASM* Mikhail A. Sokolov Eric T. Manneschmidt Materials Science and Technology Division, Oak Ridge National Laboratory, Tenn. Ductile fracture toughness testing is
More informationComposite Design Fundamentals. David Richardson
Composite Design Fundamentals David Richardson Contents A review of the fundamental characteristics of composites Stiffness and Strength Anisotropic Role of fibre, matrix and interface Composite failure
More informationSheet metal operations  Bending and related processes
Sheet metal operations  Bending and related processes R. Chandramouli Associate DeanResearch SASTRA University, Thanjavur613 401 Table of Contents 1.QuizKey... Error! Bookmark not defined. 1.Bending
More informationSEISMIC RETROFITTING TECHNIQUE USING CARBON FIBERS FOR REINFORCED CONCRETE BUILDINGS
Fracture Mechanics of Concrete Structures Proceedings FRAMCOS3 AEDIFICA TIO Publishers, D79104 Freiburg, Germany SEISMIC RETROFITTING TECHNIQUE USING CARBON FIBERS FOR REINFORCED CONCRETE BUILDINGS H.
More informationPipe Vibration and Pressure Detection
Briiel & Kjaer ffi]j W i l Pipe Vibration and Pressure Detection 13069 I CONTENTS Page Pipe Vibration Literature 1 Detection of Pressure Variations in Thin Walled Pipes by Vibration Measurement 3 Pipe
More informationSilicone Rubber Thermal Interface Materials: Applications and Performance Considerations
Silicone Rubber Thermal Interface Materials: Applications and Performance Considerations David C. Timpe Jr. Arlon Silicone Technologies Division 1100 Governor Lea Road, Bear, DE 19701 P: 8006359333 F:
More informationQuestion 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm
14:440:407 Ch6 Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm 12.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationSTRAINLIFE (e N) APPROACH
CYCLIC DEFORMATION & STRAINLIFE (e N) APPROACH MONOTONIC TENSION TEST AND STRESSSTRAIN BEHAVIOR STRAINCONTROLLED TEST METHODS CYCLIC DEFORMATION AND STRESSSTRAIN BEHAVIOR STRAINBASED APPROACH TO
More informationEXPERIMENTAL EVALUATION OF REINFORCED CONCRETE BEAM RETROFITTED WITH FERROCEMENT
Int. J. Struct. & Civil Engg. Res. 2013 Y V Ladi and P M Mohite, 2013 Research Paper EXPERIMENTAL EVALUATION OF REINFORCED CONCRETE BEAM RETROFITTED WITH FERROCEMENT Y V Ladi 1 * and P M Mohite 2 *Corresponding
More informationThe Material Properties of Cement Paste with Fly Ash Exposed to High Temperatures
The Material Properties of Cement Paste with Fly Ash Exposed to High s PAVEL PADEVĚT, ROMANA LOVICHOVÁ Department of Mechanics Czech Technical University in Prague Thákurova 7, 166 29, Prague 6 CZECH REPUBLIC
More informationCourse 1 Laboratory. Second Semester. Experiment: Young s Modulus
Course 1 Laboratory Second Semester Experiment: Young s Modulus 1 Elasticity Measurements: Young Modulus Of Brass 1 Aims of the Experiment The aim of this experiment is to measure the elastic modulus with
More informationFAILURE MODES and MATERIALS PROPERTIES. Component failures. Ductile and Brittle Fracture COMPONENT FAILURES. COMPONENT FAILURE MODES examples:
FAILURE MODES and MATERIALS PROPERTIES MECH2300  Materials Lecture 10 R. W. Truss Materials Engineering R.Truss@uq.edu.au COMPONENT FAILURES Structures lectures es on component es cause response in component
More informationA High Reliability, Stressfree Copper Deposit for FPC, Polyimide and RigidFlex
As originally published in the IPC APEX EXPO Conference Proceedings. A High Reliability, Stressfree Copper Deposit for FPC, Polyimide and RigidFlex Jason Carver Alvin Kucera OM Group Electronic Chemicals
More informationA8 Thermal properties of materials
A8 Thermal properties of materials Thermal properties the melting temperature, T m, and the glass temperature (temperatura de transição vítrea), T g, relate directly to the strength of the bonds in the
More informationA STUDY ON BONDING STRENGTH OF POLYMERIC FIBERS TO CEMENTITIOUS MATRIX
CD01006 A STUDY ON BONDING STRENGTH OF POLYMERIC FIBERS TO CEMENTITIOUS MATRIX H.R. Pakravan 1, M. Jamshidi 2, M. Latifi 3 1 M.Sc. student, Textile Engineering Department, Amirkabir University, Tehran,
More informationFourthOrder Compact Schemes of a Heat Conduction Problem with Neumann Boundary Conditions
FourthOrder Compact Schemes of a Heat Conduction Problem with Neumann Boundary Conditions Jennifer Zhao, 1 Weizhong Dai, Tianchan Niu 1 Department of Mathematics and Statistics, University of MichiganDearborn,
More informationLecture 3 Fluid Dynamics and Balance Equa6ons for Reac6ng Flows
Lecture 3 Fluid Dynamics and Balance Equa6ons for Reac6ng Flows 3. 1 Basics: equations of continuum mechanics  balance equations for mass and momentum  balance equations for the energy and the chemical
More informationFracture and strain rate behavior of airplane fuselage materials under blast loading
EPJ Web of Conferences 6, 6 42017 (2010) DOI:10.1051/epjconf/20100642017 Owned by the authors, published by EDP Sciences, 2010 Fracture and strain rate behavior of airplane fuselage materials under blast
More informationThe University of Birmingham (Live System)
The University of Birmingham (Live System) Behaviour of Structural Insulated Panels (SIPs) under both shortterm and longterm loadings Yang, Jian; Rungthonkit, Prathan Document Version Author final version
More informationINTRODUCTION TO BEAMS
CHAPTER Structural Steel Design LRFD Method INTRODUCTION TO BEAMS Third Edition A. J. Clark School of Engineering Department of Civil and Environmental Engineering Part II Structural Steel Design and Analysis
More informationNumerical Simulation of Temperature and Stress Fields in the Rock Heating Experiment
Numerical Simulation of Temperature and Stress Fields in the Rock Heating Experiment Author P. Rálek 1*, M. Hokr 1 1 Technical University of Liberec, Liberec, Czech Republic *Corresponding author: petr.ralek@tul.cz
More informationEML 5526 FEA Project 1 Alexander, Dylan. Project 1 Finite Element Analysis and Design of a Plane Truss
Problem Statement: Project 1 Finite Element Analysis and Design of a Plane Truss The plane truss in Figure 1 is analyzed using finite element analysis (FEA) for three load cases: A) Axial load: 10,000
More informationTechnology, Tehran Polytechnic, Iran. Technology, Tehran Polytechnic,Iran. Guimarães, Portugal
Cementitious Composites Reinforced With Polypropylene, Nylon and Polyacrylonitile Fibres H.R. Pakravan 1, a, M. Jamshidi 2, b,m. Latifi 3, c, F.PachecoTorgal 4, d 1 Department of Textile Engineering,
More informationNonlinear Models of Reinforced and Posttensioned Concrete Beams
111 Nonlinear Models of Reinforced and Posttensioned Concrete Beams ABSTRACT P. Fanning Lecturer, Department of Civil Engineering, University College Dublin Earlsfort Terrace, Dublin 2, Ireland. Email:
More informationMicrostructure Changes of Machined Surfaces on Austenitic 304 Stainless Steel
Microstructure Changes of Machined Surfaces on Austenitic 304 Stainless Steel Lin. Yan, Wenyu. Yang, Hongping. Jin Zhiguang Wang Abstract This paper presents a experiment to estimate the influences of
More informationThe Mechanical Properties of Glass
The Mechanical Properties of Glass Theoretical strength, practical strength, fatigue, flaws, toughness, chemical processes Glass Engineering 150:312 Professor Richard Lehman Department of Ceramics and
More informationEvaluation Of Elastic Modulus And Stress Gradient Of PECVD Silicon Nitride Thin Films
Evaluation Of Elastic Modulus And Stress Gradient Of PECVD Silicon Nitride Thin Films H. Huang 1, K. Winchester 2, J. Antoszewski 2, T. Nguyun 2, M. Martyniuk 2, B. Walmsley 1, Yinong Liu 1, X.Z. Hu 1,
More informationWaterproofing System for Wastewater Tanks in Petrochemical Industries and Refineries
Waterproofing System for Wastewater Tanks in Petrochemical Industries and Refineries Introduction Wastewater of petrochemical industries and refineries contains high amounts of emulsified aliphatic or
More informationTest Device and Method for Evaluation of Lubricants for P/M Compaction. Gerald A. Gegel Engineering SpecialistResearch Caterpillar Inc.
Test Device and Method for Evaluation of Lubricants for P/M Compaction Gerald A. Gegel Engineering SpecialistResearch Caterpillar Inc. Dr. Sydney Luk Director, Chemical Technologies Hoeganaes Corporation
More informationMachining. (Reading: Chap 8 in Kalpakjian and Schmid)
Machining (Reading: Chap 8 in Kalpakjian and Schmid) Outline Chip formation during machining Force and power requirement Mechanisms of tool wear and fatigue Types and properties of cuttingtool materials
More informationFREE VIBRATION OF SPHERICAL SHELL USING FINITE ELEMENT APPROACH
Communication Science & technology N 4. January 04 COST FREE VIBRATION OF SPHERICAL SHELL USING FINITE ELEMENT APPROACH M. BOUAZZA,, A. LAIREDJ 3, D. OUINAS 4, and A. HAMOUINE Department of Civil Engineering,
More informationAdhesion of Coatings
Adhesion of Coatings J. Baghdachi, Ph.D. Coatings Research Institute Eastern Michigan University (734) 4873192 Freshpaint@aol.com jamil.baghdachi@emich.edu Outline: What is adhesion Factors affecting
More informationExperimental assessment of concrete damage due to exposure to high temperature and efficacy of the repair system
MATEC Web of Conferences 6, 06002 (2013) DOI: 10.1051/matecconf/20130606002 C Owned by the authors, published by EDP Sciences, 2013 Experimental assessment of concrete damage due to exposure to high temperature
More informationUltrasonic Technique and Device for Residual Stress Measurement
Ultrasonic Technique and Device for Residual Stress Measurement Y. Kudryavtsev, J. Kleiman Integrity Testing Laboratory Inc. 80 Esna Park Drive, Units 79, Markham, Ontario, L3R 2R7 Canada ykudryavtsev@itlinc.com
More information